Reversible polymorphic structural transition of crown-like nickel nanoclusters and its effect on conductivity.
Maman, Manju P.; Nath, Akashdeep; Anjusree S, ?; Das, Bikas C.; Mandal, Sukhendu; Chemical communications (Cambridge, England) 57 (2021) 2935–2938; doi:10.1039/d1cc00402f

data_7127956
_publ_section_title
;
 Reversible polymorphic structural transition of crown-like nickel
 nanoclusters and its effect on conductivity.
;
_journal_issue                   23
_journal_name_full
'Chemical communications (Cambridge, England)'
_journal_page_first              2935
_journal_page_last               2938
_journal_paper_doi               10.1039/d1cc00402f
_journal_volume                  57
_journal_year                    2021
_chemical_formula_sum            'C48 H54 N0 Ni3 S6'
_chemical_formula_weight         999.40
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2021-01-03 deposited with the CCDC.	2021-02-15 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 91.641(5)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.329(5)
_cell_length_b                   12.521(6)
_cell_length_c                   32.774(15)
_cell_measurement_reflns_used    9509
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      26.372
_cell_measurement_theta_min      1.243
_cell_volume                     4647(4)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker SAINT'
_computing_data_reduction        'Bruker APEX2'
_computing_molecular_graphics    'Mercury (Macrae <i>et al.</i>, 2008)'
_computing_publication_material
'WINGX (Farrugia, 2014) and PLATON(Spek, 2009)'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1930
_diffrn_reflns_av_unetI/netI     0.1643
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       40
_diffrn_reflns_limit_l_min       -40
_diffrn_reflns_number            45697
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.372
_diffrn_reflns_theta_min         1.243
_exptl_absorpt_coefficient_mu    1.505
_exptl_absorpt_correction_T_max  0.929
_exptl_absorpt_correction_T_min  0.714
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   SADABS-2014/5
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    1.428
_exptl_crystal_description       plate
_exptl_crystal_F_000             2088
_exptl_crystal_size_max          0.240
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.050
_refine_diff_density_max         1.158
_refine_diff_density_min         -1.628
_refine_diff_density_rms         0.396
_refine_ls_extinction_coef       0.0205(13)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_goodness_of_fit_ref   1.167
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     515
_refine_ls_number_reflns         9509
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.167
_refine_ls_R_factor_all          0.1924
_refine_ls_R_factor_gt           0.1093
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1005P)^2^+29.0027P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2651
_refine_ls_wR_factor_ref         0.3115
_reflns_Friedel_coverage         0.000
_reflns_number_gt                5083
_reflns_number_total             9509
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d1cc00402f2.cif
_cod_data_source_block           NiPET_1
_cod_depositor_comments
'Adding full bibliography for 7127956--7127957.cif.'
_cod_original_sg_symbol_H-M      'P 21/n'
_cod_database_code               7127956
_shelx_shelxl_version_number     2018/3
_shelx_estimated_absorpt_t_min   0.714
_shelx_estimated_absorpt_t_max   0.929
_shelx_res_checksum              88197
_shelx_hkl_checksum              20456